Presentation on theme: "MATERIAL R&D FOR HIGH-INTENSITY PROTON BEAM TARGETS PROGRESS REPORT Nicholas Simos, BNL January 4, 2005."— Presentation transcript:
MATERIAL R&D FOR HIGH-INTENSITY PROTON BEAM TARGETS PROGRESS REPORT Nicholas Simos, BNL January 4, 2005
GOAL SEARCH for and evaluate under irradiation environment NEW materials or composites that appear to hold the answer the problem of survivability as high power targets by exhibiting unusually high strength, very low thermal expansion or high ductility
Experimentation with Graphite & Carbon-Carbon Targets (BNL E951)
Graphite vs. Carbon-Carbon – A Clear Choice ….. really?
Irradiation of Super Invar Alloy at BNL to Assess Coefficient of Thermal Expansion and Mechanical Properties
Effect of Irradiation on the Ultimate Stress of Super Invar based on the BNL Test
Solid Target Option: Super-Invar Irradiation Study WHY STUDY super Invar ? High-Z with low CTE (0-150 o C) How is CTE affected by radiation? What happens to other important properties?
Super-Invar Irradiation Study – Temperature Effects
PHASE II -TARGET MATERIAL R&D Carbon-Carbon Composite (BNL) Toyota “Gum Metal” (KEK) Graphite (IG-43) (KEK) AlBeMet (BNL) Beryllium (BNL) Ti Alloy (6Al-4V) (SLAC) Vascomax (BNL) Nickel-Plated Aluminum Used in the NUMI Horn (BNL-FNAL-KEK)
WHAT IS OF INTEREST TO US IN POST-IRRADIATION PHASE Resilience in terms of strength/shock absorption CTE evaluation Stress-strain Fatigue Fracture Toughness and crack development/propagation Corrosion Resistance De-lamination (if a composite such as CC or plated HORN conductor) – Use of ultrasonic technology to assess changes Degradation of conductivity Other tests are also in the planning for scrutiny of the successful candidates (laser induced shock and property measurements)
Carbon-Carbon Composite Target Temp.% elongation 23 o C0% 200 o C-0.023% 400 o C-0.028% 600 o C-0.020% 800 o C0% 1000 o C0.040% 1200 o C0.084% 1600 o C0.190% 2000 o C0.310% 2300 o C0.405%
The Wonders of Gum Metal (soon in peppermint flavor !!)
Tensile and CTE Specimen Design
Tensile and CTE Specimen Assembly into the Target Box During Irradiation
TARGET BOX ASSEMBLY DETAILS
GUM Metal Layout in Irradiation Box Nickel-Plated Aluminum Specimens (NUMI Horn Material) Embedded Nickel foils used for radiography profile
Estimation of Irradiation Temperature Using Aluminum Plate into the BLIP Irradiation Facility and Temperature Sensitive Paint (TSP) Experiment Simulation
Activation & Beam profile Assessment
HOT CELL Specimen Analysis Dilatometer Remotely operated Tensile Tester
Preliminary Results from Testing Irradiated Specimens at the BNL Hot Cell Facility NOTE that just a few of the tested specimens of each material is presented in the following graphs. While most of the irradiated samples have been tested, no correlation with the specimen activation has been made. Further, the non- irradiated specimen testing is incomplete (this will provide a better estimate of what the non-irradiated stress values, such as yield and ultimate, were prior to irradiation) The Stress-Strain Curves generated are from RAW data with no adjustment for “effective” strain gauge (results shown assume that only the 6mm neck-down section of the specimen contributes to the total extension of the specimen) Given that the position of the proton beam spot was slightly off centered, a second level of correlation will be performed based on the location within the 6mm gauge (neck-down) where rupture occurred.